Grátis

8 pág.

# Predicted-Superconductivity-in-the-Electride-Li5C

- Denunciar

## Pré-visualização | Página 2 de 7

30 generations of crystal structures at 200 GPa with up to four formula units, totalizing 1500 structures constrained within all space groups. For each generation, 60% of the structures with the smallest enthalpies are used to construct the next generation, while 40% are formed by random structures. The insertion of random structures prevents premature convergence in the PSO algorithm. Each structure is optimized in the VASP package33 using Perdew−Burke−Ernzerhof (PBE) exchange function- als34 and projector augmented wave (PAW) pseudopoten- tials35 for lithium and carbon with valence configurations 1s2 2s1 2p0 and 2s2 2p2, respectively. The kinetic energy cutoff for the wave function was 650 eV and the k-spacing tag used was 0.25 Å−1 (VASP input tag). It means that the number of k- points in any reciprocal lattice vector is given by = | | → N b kmax(1, / spacing)i , where πδ⃗ = ⎯ →⎯⎯ b a 2i ij ij and ÷ ◊÷÷aij are the real lattice vectors. The k-grid is a Monkhorst−Pack mesh centered at the γ point. After the search, we optimized again the five structures with the lowest enthalpies found (Li5C in Cm, C2/m, Imm2, Immm, and P6/mmm symmetries), but at this, a finer k-grid (k-spacing = 0.08) was used. For the best structures found, phonon frequencies were analyzed using density functional perturbation theory (DFPT)36 as imple- mented in the Quantum ESPRESSO (QE) package.37,38 Only Li5C (P6/mmm) emerges as a potential stable phase, the other structures were found to be unstable. Therefore, we present Li5C as a potential global phase at 200 GPa (see structural parameters Table S1 in the Supporting Information). To validate the pseudopotential used at high pressure, the present calculations were compared with the pressure versus volume curve for Li5C using the LAPW (linearized augmented plane wave) methodology as implemented in the ELK code.39 The Li5C structure was relaxed (unit cell and atom positions) by QE in the range from 30 to 250 GPa with steps of 2 GPa. The energy of each relaxed structure was also calculated using the LAPW method, and as a result, the pressure versus volume curve for both methods was compared, as illustrated in Figure S1, showing good agreement between those two method- ologies. For phonon and electron−phonon calculations, we also used PAW pseudopotentials in the GGA approximation at the PBE level, considering three electrons in the valence of lithium (1s2 2s1 2p0) and four electrons in the valence of carbon ([He] 2s2 2p2). The kinetic energy cutoff for wave functions was 70 and 350 Ry for charge density cutoff. We used a 28 × 28 × 25 k- grid Monkhorst−Pack mesh centered at the γ point and a 7 × 7 × 5 grid for q-points. Since the calculations for electron− phonon matrix elements require very dense grids, the double grid technique40 implemented by Wierzbowska et al. in QE was used. This approach has been used successfully in many articles.41−44 In this approximation, the electron−phonon matrix elements are calculated in a 28 × 28 × 25 k-grid and interpolated in a denser k-grid, 56 × 56 × 50. The coupling parameter λ is calculated by the Eliashberg spectral function α2F(ω), which is built from electron−phonon matrix elements. The sigma broadening parameter was 0.01 Ry, which approximates the zero-width limits in the calculation of Tc. A 65 × 65 × 65 k-grid was used for DOS and Fermi surface calculations. To calculate Tc, we used the McMillian formula modified by Allen−Dynes22 as follow ∫λ α ωω ω= ω F2 ( ) d 0 2 max (1) and Tc is given by l moo noo | }oo ~oo ω λ λ μ λ = − + − * + T f f 1.2 exp 1.04(1 ) (1 0.62)c 1 2 log (2) where ωlog, f1, and f 2 are l mo no | }o ~o ∫ω λ α ω ω ω ω= ω F exp 2 ln( ) ( ) dlog 0 2max (3) i k jjjj y { zzzz λ μ = + + * f 1 2.46(1 3.8 )1 3/2 3 (4) i k jjjjjj y { zzzzzz λ ω ω λ μ = − + + + * f 1 (1 / ) 3.312(1 6.3 )2 2 2 log 2 2 (5) and ω2 is ∫ω λ α ω ω ω ω= ω F1 2 ( ) d2 0 2 2max2 (6) The McMillian formula, as modified by Allen−Dynes, is obtained with f1·f 2 = 1, otherwise, if f1 and f 2 are calculated as in eqs 4 and 5, we have a “full” Allen−Dynes formula. Figure S2 shows how Tc changes when the Coulomb pseudopotential μ* varies in the range of 0.10−0.16. This paper also presents calculations on the hypothetical (Li5C) + crystal. Since the periodic system must have a neutral charge to avoid infinite energy repulsion by replication of the unit cell, Quantum ESPRESSO inserts a compensating jellium The Journal of Physical Chemistry C pubs.acs.org/JPCC Article https://doi.org/10.1021/acs.jpcc.1c02329 J. Phys. Chem. C 2021, 125, 8899−8906 8900 http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf http://pubs.acs.org/doi/suppl/10.1021/acs.jpcc.1c02329/suppl_file/jp1c02329_si_003.pdf pubs.acs.org/JPCC?ref=pdf https://doi.org/10.1021/acs.jpcc.1c02329?rel=cite-as&ref=PDF&jav=VoR background to remove energy divergences in case the cell is charged in a periodic system. It is important to note that this homogeneous background charge density is not included explicitly in the calculation of the total charge density in the self-consistency solution. This procedure is equivalent to adding a negative potential to compensate for the energy divergence. ■ RESULTS AND DISCUSSION Li5C is shown in Figure 1 where two perspectives of its structural phase are presented. Li5C crystallizes in the hexagonal P6/mmm space group and according to Wyckoff positions, it has two inequivalent lithium sites and one carbon site. Figure 1a shows lithium atoms at 4h site (1/3, 2/3, 0.782) (green atoms) and carbon at 1a site (0, 0, 0) (brown atoms). Figure 1b displays another perspective and adds Li atoms at 1b site (0, 0, 1/2) (for more structural parameters, see Table S1 in the Supporting Information). Phonon dispersion curves of Li5C throughout high sym- metrical q-points in the first Brillouin zone at various values of pressure (40, 50, 125, 175, 200, 210, and 230 GPa) were calculated and are shown in Figures S3 and S4 in the Supporting Information. The absence of imaginary frequencies in the range of 50−210 GPa indicates stability for Li5C in P6/ mmm symmetry. In this material, stability is induced by pressure. However, energy and phonon analysis at 0 K are limited by the lack of statistical fluctuation. Therefore, to overcome this difficulty, we also employed Car and Parrinello molecular dynamics45 with a Nose−́Hoover thermostat,46 thus simulating 384 atoms in the canonical ensemble (a supercell with 4 × 4 × 4 dimensions) to further ascertain the stability of the structures. The result is illustrated in Figure 2, in which root-mean-square deviation (RMSD) calculated by the atomic displacements shows large stability. For instance, time- averaged RMSD values, compared to perfect structures at 0 K and 200 GPa, achieve 0.08, 0.09, and 0.12 Å at temperatures of 50, 150, and 300 K, respectively; therefore, Li5C in the P6/ mmm phase maintained its stability even at 300 K simulation. Molecular dynamics calculations were performed in different situations: (i) The simulation starts at 200 GPa and after thermalization at 300 K, the pressure reaches an average of 203.5 GPa (see Figure S4b and Video in the Supporting Information). The same procedure is repeated for thermal- ization at 50 and 150 K. (ii) Simulations start at 50 GPa and 300 K and achieve a pressure of around 51.2 GPa after thermalization (Figure S5 in the Supporting Information). In these calculations, the size of the supercell was taken to be large enough to guarantee statistical fluctuations and consistent results when compared with the present DFT calculations. In summary, even assuming